Abstract
Development of onchip integrated carbonbased optoelectronic nanocircuits requires fast and noninvasive structural characterization of their building blocks. Recent advances in synthesis of single wall carbon nanotubes and graphene nanoribbons allow for their use as atomically precise building blocks. However, while cataloged experimental data are available for the structural characterization of carbon nanotubes, such an atlas is absent for graphene nanoribbons. Here we theoretically investigate the optical absorption resonances of armchair carbon nanotubes and zigzag graphene nanoribbons continuously spanning the tube (ribbon) transverse sizes from 0.5(0.4) nm to 8.1(12.8) nm. We show that the linear mapping is guaranteed between the tube and ribbon bulk resonance when the number of atoms in the tube unit cell is \(2N+4\), where \(N\) is the number of atoms in the ribbon unit cell. Thus, an atlas of carbon nanotubes optical transitions can be mapped to an atlas of zigzag graphene nanoribbons.
Introduction
Singlewalled carbon nanotubes (SWCNT) and monolayer graphene nanoribbons (GNR) are quasionedimensional nanostructures of graphene that are considered as key building blocks for onchip integrated carbon optoelectronics^{1,2,3}. The ultimate goal of onchip integration requires a deep understanding of the structurefunction interrelations and a perfect geometrical control of the building blocks. Significant advancements in the synthesis of graphene ribbons with atomic precision have been observed in recent years^{4,5}, whereas a comprehensive progress has been achieved in production of monochiral carbon nanotubes^{2,6,7}. This development has partially eliminated both the edge quality issue of graphene nanoribbons and the chirality problem for carbon nanotubes. At the same time, considerable effort has been directed towards relating SWCNT optical properties for different polarization of radiation with SWCNT chirality and diameter^{8,9,10,11,12,13,14,15,16}.
A standard way of presenting diameter dependence of SWCNT optical resonances polarized parallel to the tube axis is Kataura plot^{8}. This plot has been both measured experimentally^{9,17} and reproduced numerically in semiempirical and abinitio calculations^{18,19,20}. Several interpolating formulas have been proposed for the description of the SWCNT Kataura plot^{10,11,12}. The Kataura plot for ribbons, however, cannot be approached in the same way as Kataura plot for tubes because of two main reasons: (i) the different physical mechanisms of SWCNT and GNR synthesis and (ii) a huge variety of GNR edges, which impedes the development of the GNR standard classification, thereby leading to different naming conventions used in experimental and theoretical studies^{21,22,23}. Limiting our consideration to the symmetric nanoribbons with zigzag and armchair edges, we should notice that even these two types of GNRs are not yet well studied and understood. In particular, no Kataura plot has been reported for these graphene nanoribbons, although such plot would be practical for the fast and noninvasive ribbon width characterization, especially in those synthesis methods that provide flexible control of the ribbon width, such as catalytic writing, nanolithography, plasma etching, tube unzipping or epitaxial growth on sidewalls of SiC^{24,25,26}.
The optical properties of armchair GNRs (AGNRs) have been intensively studied theoretically^{27,28,29,30,31,32,33,34,35,36} and more recently experimentally^{37,38}, nevertheless the absorption peak dependence on the ribbon width is not yet complete. Hitherto, rather narrow energy or width ranges have been reported. The width dependence of the first (\({E}_{11}\)) and the second (\({E}_{22}\)) singleelectron excitation was exemplified for 0.3–3 nm widths^{29} while the exciton \({E}_{11}\) was studied in the AGNRs of 0.4–4 nm widths^{32}. The \({E}_{22}\) and \({E}_{33}\) excitons were also reported for the similar width ranges^{33,34,35}. Recently, an analytical width dependence has been proposed for \({E}_{11}\) exciton of semiconducting AGNRs^{36}. Even so, none of these previous works have provided a proper comparison of the AGNR optical resonances with those of zigzag SWCNTs, whereas such comparative analysis is highly desirable for a reliable optical nanodevice and nanocircuit engineering. Joint analysis of several previous studies attempting to compare zigzag SWCNTs and AGNRs indicates that Kataura plots for these ribbons could be the replica of that plot for zigzag SWCNTs. As shown within the tightbinding model, the electronic energy bands of zigzag SWCNT\((n,0)\) duplicate the bands of the AGNR\((w)\) when \(n=w+1\), where \(n\) is the chiral or diameter index of the tube and \(w\) is the width index of the ribbon^{39,40}. Similar correspondence takes place for the optical transition matrix elements^{41,42}, leading to a perfect alignment of the singleelectron optical absorption peaks of some SWCNTs and corresponding AGNRs^{40}. Moreover, this alignment should not be disordered by excitonic effects since Loudon’s model provide the same exciton binding energy for two structures of the same transverse size^{43}. Thus, Kataura plot for AGNRs could, in principle, replicate that plot for zigzag SWCNTs.
The situation is more complicated with zigzag graphene nanoribbons (ZGNRs). These nanoribbons are famous for their edge states^{44,45,46}, whose origin is traced back to polyacetylene^{47,48}. Optical properties of ZGNRs have been studied theoretically within the first principles and tightbinding models^{27,28,30,40,49,50,51,52} and experimentally with some edge modifications^{53}. However, the majority of these studies are focused on the effect of the edge states and on few selected ribbons. Only few works attempt to consider a wide range of ZGNRs. The lowest five optical transitions have been reported for wide ribbons of 12.8–76.7 nm^{30}. This study, however, omits the relation of these wide ribbon optical transitions to the transitions of armchair SWCNTs. The width dependence for the first four optical transitions is presented for narrow ZGNRs of 0.5–4.5 nm in ref. ^{49}. These results are compared to the transition energies of armchair SWCNTs through the ratio \({E}_{11}:{E}_{22}:{E}_{33}:{E}_{44}\). However, the calculated optical resonance energies in ref. ^{49} are the energy differences between the van Hove singularities symmetrically placed with respect to the intrinsic Fermi level. Associating these energies with the optical resonances contradicts to the optical selection rules^{30,31,52,54}. Not only are the selection rules different for ZGNRs and armchair SWCNTs but also their energy bands cannot be aligned. Nevertheless, a hidden correlation between the optical absorption resonances of several ZGNRs and armchair SWCNTs has been reported in the nearestneighbor tightbinding model^{40,52}. Therefore, ZGNRs and armchair SWCNTs deserve primary consideration to provide an entry point for a general understanding of the optical interrelations between SWCNTs and GNRs.
In this paper, we study the interrelations between optical absorption resonances in ZGNRs and armchair SWCNTs for the parallel polarization of the incident light. Accounting for the exchange and correlation effects, we analyze the degree of linear correlation and alignment between the optical resonances as a function of the tube diameter and ribbon width. We reveal a \(2N+4\)rule according to which the maximum of the linear correlation and alignment is observed when the effective width of the ribbon is equal to the half of the tube circumference, which is equivalent to the number of carbon atoms in the armchair SWCNT unit cell being \(2N+4\), where \(N\) is the number of carbon atoms in a zigzag GNR. We apply this rule to the atlas of SWCNTs^{11} and predict the resonance energies for the bulkbulk transitions of ZGNRs.
Results
Optical absorption of armchair SWCNTs and zigzag GNRs
In this letter, we use the integers \(n\) and \(w\) as the tube diameter and ribbon width indices, respectively^{40}. These indices can be readily converted to the actual diameter of the tube \(d\) and width of the ribbon \(W\) as follows: \(d=\sqrt{3}an/\pi\) and \(W=\sqrt{3}aw/2\), with \(a=2.46\) Å being the graphene lattice constant. The intensity of the absorption as a function of the structure transverse size and excitation energy is presented in Fig. 1 (see Methods for details). These graphs are an analog of the celebrated Kataura plots^{8,9} for SWCNTs with a difference that these diagrams only present the absorption resonances for the ZGNRs (Fig. 1a, b) and armchair SWCNTs (Fig. 1c, d). From multiple SWCNT experimental studies^{9,10,11,12}, the first four^{10,12} and even higher^{11} absorption peaks can be recovered by the interpolating formulas. However, no experimental data and interpolating formulas are available for the zigzag GNRs. Comparing the results in Fig. 1a, c obtained for the tubes and ribbons in the nearestneighbor Partoens 2006^{55} tightbinding model (TBM), one can clearly identify two regions in the absorption spectra of the ribbons. The first region at \(\hslash \omega \ \gtrsim \ 3\) eV has a strikingly similar pattern to the intensity plot of the tubes, while the second region at \(\hslash \omega \ \lesssim \ 3\) eV contains additional peaks converging to the threshold of \({t}_{1} \approx 3\) eV as the ribbon width decreases. These additional resonances originate from the edge states (see Supplementary Fig. 3 in Supplementary Note 2), and they are noticeably weaker in intensity with the exception of the lowest energy resonance, which is comparable in intensity to the strongest resonance situated at \(2{t}_{1} \approx 6\) eV. The high energy resonance at \(2{t}_{1} \approx 6\) eV sets the upper boundary for the diverse peak structure in absorption of both tubes and ribbons. It represents the persistent \(\pi\)plasmon that is routinely observed in all graphitic materials^{56}. By analogy, the much weaker edge \(\pi\)plasmon at \({t}_{1} \approx 3\) eV sets the upper boundary for the edge resonances in ZGNRs (see also Supplementary Fig. 3 in Supplementary Note 2). The intensity plots show that all the intensity curves, which split from the 6 eV in the ZGNR, i.e., those which correspond to the bulktobulk state transitions, have counterparts in the intensity plot of the armchair SWCNTs. However, the lowest energy absorption resonances of the armchair SWCNTs do not have a counterpart among the bulk–bulk resonances in the ZGNR absorption spectra.
Advancing to the multiparameter TBM—with parameters fitted to the Density Functional Theory (DFT) and given in Table 1—we notice in Fig. 1b, d that the main features of the singleparameter model still persist. The boundary between the pure bulk and the bulkedge transition regions in the ribbons is distinguishable for narrow ribbons but gradually diffuses for wider ones. The \(\pi\)plasmon resonance is clearly identified with a red shift to \(\sim\!4.0\) eV for both the armchair SWCNTs and ZGNRs (see also Supplementary Figs. 4 and 6). When this resonance is observed for graphene^{57,58,59}, the shift between the experimental and theoretical data is typically attributed to the excitonic effects^{57,58} or the excitonic effect with Keldysh dielectric confinement and an influence of the substrate^{59}. The energy of the \(\pi\)plasmon resonance in our calculations is in good agreement with the interpolating formula from ref. ^{11} (see Supplementary Fig. 8c in Supplementary Note 3), which provides an evidence that indeed the multiparameter models used here have partially incorporated the manybody effects such as Coulomb electronelectron interactions. In contrast to the diffused edgebulk transitions resonances found at \(\sim\!2\) eV in Fig. 1b, the bulkbulk resonances are less affected by the stated manybody effects. Although the bulk–bulk resonances are squeezed within the range of 0–4 eV due to the manybody effects, the peaks preserve a pattern that exhibits the same number of curves for both SWCNTs and ZGNRs when \(n \approx w\). This implies that the energies of the optical absorption resonances in armchair SWCNTs and ZGNRs can be correlated and aligned. These alignment patterns and correlation signature motivate us to study this certain feature in more detail.
Linear correlation coefficient analysis
In order to scrutinize a full picture of the existing correlations between the energies of optical resonances in the tubes and ribbons, we have calculated the linear correlation coefficient (LCC) for all possible pairs of SWCNTs and ZGNRs with \(n=4,5,\ldots ,60\) and \(w=2,3,\ldots ,60\) (see Methods for details). Two types of LCC are of interest: (i) the LCC between the full set of absorption resonances in ZGNR, including edgetobulk transitions, and in armchair SWCNT and (ii) the LCC between bulkbulk ZGNR resonances and armchair SWCNTs resonances. The type (i) and (ii) datasets cannot be obtained by analysis of the full absorption spectra of ZGNRs with the peak selection algorithm presented in Methods because it is not selective with respect to the edgetobulk or bulk–bulk nature of the optical resonances. An effective approach to isolating such datasets is to apply the peak selection algorithm to the bulk absorption spectra obtained by exclusion of the edge states from the summation in the optical absorption (see Eq. (2) in Methods). As one can clearly see from Supplementary Figs. 3 and 4 in Supplementary Note 2, the inclusion or exclusion of the edge states from the summation does not affect the energies of the bulkbulk resonances. Therefore, this procedure is equivalent to the selection of the bulk absorption resonances from the full absorption spectra. In both datasets (i) and (ii), the lowest energy resonance of the armchair SWCNT spectra is excluded being the only tube resonance with no counterpart bulk resonance in the ZGNR absorption spectra (see Supplementary Figs. 5 and 6 in Supplementary Note 2). In Fig. 2, the LCC maps at the threshold \(r\ > \ {r}_{{\rm{th}}}\) for the single (Fig. 2a–f) and multi (Fig. 2g–l) parameter TBMs are compared with the theoretical reference line \(n=w+1\) obtained by matching the transverse momenta of tube and ribbon electrons^{52}. Such matching is achieved by equating the transverse momenta \(\theta\) quantized in the two nanostructures by the secular equations: \(\cos \left(n\theta /2\right)=1\) (for tube) and \(\sin \left(w\theta \right)+2\cos \left(k/2\right)\sin \left[(w+1)\theta \right]=0\) (for ribbon). We note that ZGNR secular equation depends on the electron longitudinal momentum \(k\). By setting \(k\to 0\), which corresponds to the approximate alignment of the ribbon energy bands to the tube ones at the center of the Brillouin zone^{61}, the secular equation for the ribbon has solution \({\theta }_{{\rm{r}},j}=\pi j/\left(w+1\right)\), while the solution for the tube is \({\theta }_{{\rm{t}},j}=\pi j/n\). The reference line is derived by setting \({\theta }_{{\rm{r}},j}={\theta }_{{\rm{t}},j}\). Allowing the edgetobulk state transitions in Partoens2006 TBM and including of the corresponding resonances into the datasets show a significant deviation from the reference line as observed from Fig. 2a–c. However, the exclusion of the edge state optical resonances from the datasets leads to a perfect agreement with the reference line shown in Fig 2d–f. It follows from Fig. 2g–i that in the LCC maps obtained from the multiparameter TBMs, the high LCC regions form irregular sparse patterns above the reference line if the edge states are involved in the optical absorption. However, a good agreement with the reference line is restored by retaining only the bulk–bulk optical transitions. In summary, the LCC maps in Fig. 2 confirm that the linear relation is warranted for the twodimensional dataset of optical resonance energies of the armchair SWCNT\((n,n)\) and ZGNR\((w)\) pair when \(n=w+1\). Also, a more detailed comparison between the optical absorption spectra of the selected tuberibbon pairs (see Supplementary Figs. 5 and 6 in Supplementary Note 2) suggests that the optical resonances are not only linearly related but also precisely aligned.
Alignment coefficient analysis
We present in Fig. 3 the maps of the alignment coefficient (AC) \({L}_{{\rm{c}}}\) discriminated at several thresholds \({L}_{{\rm{c}}}\ > \ {L}_{{\rm{c,th}}}\) and compared with the reference line \(n=w+1\) (see Methods). The regions of high AC obtained from the singleparameter TBM shown in Fig. 3a–d are narrower than those of the multiparameter TBMs shown in Fig. 3e–h. The broadening of the high AC region in Fig. 3e–h is explained by the squeezing of the absorption resonances presented in Fig. 1. In both types of TBMs, the maximum degree of alignment is observed in the tuberibbon pairs \(n=w+1\) between the bulk ZGNR and armchair SWCNT resonances. Comparing the panels c–d and g–h of Fig. 3, it can be observed that the degree of alignment in the fitted TBMs is slightly less than that in the nearestneighbor TBM. Nevertheless, in both cases the AC value exceeds 0.99, which corresponds to the sample variance \(\sigma =\beta\,\mathrm{ln}\left({L}_{{\rm{c}}}\right)=0.01\) eV\({}^{2}\).
2N+4rule of armchair SWCNTs and ZGNRs
The high degree of linear correlation and alignment between the optical resonances in the fitted TBMs presented in Figs. 2 and 3 implies that similar results should be observed for the absorption spectra calculated with the DFT wavefunctions. It can be seen in Fig. 4a, b that similar to ref. ^{62} the DFT and fitted TBM absorption spectra are in full agreement. It is also seen in Fig. 4a, b that bulk spectra of ZGNRs can be obtained from full spectra by exclusion of the edge states without affecting positions of the bulk resonances. The match between the DFT and TBM absorption spectra for SWCNTs is better than that between the spectra for ZGNRs due to the slight deviation of the TBM energy bands from the DFT ones (see Supplementary Fig. 1 in Supplementary Note 1). Also, Fig. 4a, b indicates that the LCC and AC calculated for the DFT absorption spectra are larger than the corresponding coefficients for the fitted TBMs absorption spectra. Our calculations for the points presented in Fig. 4c show that for the DFT data LCC \(r=0.99987\) and AC \({L}_{{\rm{c}}}=0.99934\), while for the fitted TBM data we have LCC \(r=0.83365\) and AC \({L}_{{\rm{c}}}=0.98644\).
The correlation and alignment found for the tubes and ribbons mean that the \(n=w+1\) tuberibbon pairs represent a rule of geometrical matching for the optical resonance alignment. As illustrated in Fig. 4d, the number of carbon atoms in the tube unit cell for these specific pairs is expressed via the number of atoms in the ribbon unit cell \(N\) as \(2N+4\).
An atlas of ZGNR absorption resonances by linear mapping
The revealed regularity can be employed to predict experimental optical absorption resonances for zigzag GNRs, which have not been explored experimentally yet. We present in Fig. 5 the linear mapping between the optical absorption resonances of armchair SWCNTs and ZGNRs carried out with the parameters extracted from the fitted TBMs in Table 1 (see Supplementary Figs. 7 and 8 in Supplementary Note 3). The data points for ZGNRs presented by the large red open circles in Fig. 5 are described by the following equation:
where \({\xi }_{{\rm{R}},1}=2.83\), \({\zeta }_{{\rm{R}},2}=0.98\), \({\xi }_{{\rm{R}},3}=7.42\) eV, \({\zeta }_{{\rm{R}},4}=0.03\) eV and \({E}_{{\rm{aSWCNT}}}\) is given by the interpolating formula from ref. ^{11}. The calculation for the nanotube with the diameter index \(n\) gives the resonance energy for the nanoribbon with width index \(w=n1\). These energies are the optical resonances predicted for an atlas of ZGNRs. Eq. (1) should provide a more precise estimate for ZGNRs with width index \(w\ge 9\), since only the regular part of the linear mapping coefficients for \(n\ge 10\) was used in their fitting (see Supplementary Fig. 7 in Supplementary Note 3). We have also plotted in Fig. 5 the green solid curves given by the Jiang et. al. fitting formula^{49}. The formula provides the resonance energies of ZGNRs, which are close to the atlas obtained by mapping from the armchair SWCNTs. This is especially true for the first bulk resonance. In order to verify if this is indeed possible, we have performed similar calculations within the ZGNR (av.) TBM and have included these results to Fig. 5 as small open black circles. The black data points and green solid curves show scaling with the ribbon width that is deceivingly similar to that of actual absorption resonances given by large red open circles of the ZGNR atlas. However, the optical resonances allowed by selection rules must originate from the van Hove singularities that are asymmetrically rather than symmetrically situated with respect to the Fermi level. Therefore, we recommend to follow the atlas in order to avoid the mistakes in the optical resonance energy estimation. Based from the results presented above, we should mention that the linear mapping similar to Eq. (1) should be possible between the armchair GNRs and zigzag SWCNTs due to their straightforward similarity in both electronic and optical properties^{39,40,41,42}.
Discussion
In addition to the atlas application, the \(2N+4\)rule for the optical resonance alignment can be utilized for building functional carbon materials on a molecular scale and for designing multifrequency resonant optoelectronic devices. It is also important to note that the geometrical match within the tuberibbon pairs can be a source of undesired crosstalk between the different parts of complex optoelectronic circuits when the optical resonance line width is larger than the standard deviation \(\sqrt{\beta\,\mathrm{ln}\left({L}_{{\rm{c}}}\right)}\) estimated from the AC. Such a crosstalk can manifest itself in the cloaking of the hybrid GNR@SWCNT systems^{63,64}, making one of the constituents invisible for optical characterization in a specific spectral range. Therefore, special care must be taken in the interpretation of measurements for such hybrid systems.
To conclude, we have revealed that the optical resonances of armchair single wall carbon nanotubes and zigzag graphene nanoribbons in parallel polarization of the incident light are related by a linear transformation when \(n=w+1\), where \(n\) is the diameter(chiral) index and \(w\) is the width index. The \(n=w+1\) relation is equivalent to the \(2N+4\)rule for the number of carbon atoms in a nanotube unit cell, where \(N\) is the number of atoms in a ribbon unit cell. This rule is valid not only in the simple nearestneighbor tightbinding model but also in more complicated models following the density functional theory calculations and simulating the electron exchange and correlation effects with several phenomenological parameters. Despite the different topology of the structures (cylindrical and planar), optical selection rules and notorious edge states, a high degree of alignment coefficient (\(>0.99\)) is found for the bulkbulk transitions of ZGNR\((w)\) and for all but the first \(\pi\)electron optical resonances of armchair SWCNT\((n,n)\), when the \(2N+4\)rule is fulfilled. This allows one to predict the bulkbulk transitions of zigzag GNRs by mapping the atlas of armchair SWCNTs optical transitions of Liu et al.^{11}. Finally, we note that the atlas for nanoribbons can be further expanded to include the armchair GNR optical resonances, since similar mapping should be possible between the zigzag SWCNTs and armchair GNRs. Also, it would be interesting to investigate the effects of external electric and magnetic fields^{65} which—as we anticipate—could be used to tune the degree of correlation and alignment between the optical absorption resonances.
Methods
DFT calculations
All density functional theory (DFT) calculations were performed in Quantum Espresso package using the normconserving pseudopotential with PerdewBurkeErnzerhof exchange and correlation^{66}. In these calculations, we used 40 Ry kinetic energy cutoff for the plane wave expansion and set the vacuum distances between periodic images of the structures to be about twice the transverse size of the structure (width for the ribbons and diameter for the tubes). In the majority of the bandstructure calculations, the Brillouin zones were sampled with \(30\,\times\,1\,\times\,1\) uniform \(k\)points mesh. For ZGNR(20) and SWCNT(21,21), we used a denser mesh of \(60\,\times\,1\,\times\,1\) \(k\)points and the kinetic energy cutoff of 100 Ry. For the sake of tightbinding model (TBM) parameters fitting, in all cases we used the nonrelaxed ideal geometries of the structures (see Supplementary Discussion). The singleelectron optical absorption spectra based on DFT wavefunctions were calculated within the pw2gw package of Quantum Espresso.
Tightbinding calculations
In the tightbinding calculations, we first followed an idealized picture where a singleparameter tightbinding model (TBM) was used for both tubes and ribbons by setting the nearestneighbor hopping integral \({t}_{1}=3.12\) eV (Partoens 2006)^{55}. Then, for zigzag GNRs, 6 TBM parameters were fitted to the DFT results to facilitate the study taking into account exchange and correlation effects for a wide range of transverse sizes. The fitted parameters are given in Table 1. For armchair SWCNTs, we used 7 tightbinding parameters reported by Reich et al. (Reich 2002)^{60} because they perfectly describe the calculated DFT bandstructures of the carbon nanotubes (see Suplementary Note 1). These parameters are also given in Table 1.
For all TBMs, the singleelectron optical absorption spectra for the incident light polarized along the longitudinal axis of the nanoribbon or nanotube were calculated using the gradient approximation for the velocity operator^{67}: \(v=\partial H(k)/\partial k\). Then, with this operator the interband absorption is calculated as follows^{27,56}:
where \({\Psi }_{{\rm{c(v)}},i(j)}\) are the eigenvectors of the generalized eigenproblem \(H\Psi =ES\Psi\) and \(\delta (E)\) is the Dirac delta function that is replaced in numerical calculations by a Gaussian function with broadening \(\alpha\) to model a range of deexcitation processes, i.e., \(\delta (E)\to \exp \left\{{E}^{2}/{\alpha }^{2}\right\}\). Eq. (2) assumes the zero temperature. The summation \({\sum }_{k}\) in Eq. (2) runs through the Brillouin zone sampled with 1000 \(k\)points for the energy bandstructure calculations. The broadening of a single transition was chosen to be \(\alpha =0.03\) eV. This broadening corresponds to relaxation time \(\tau =0.14\) ps that is a medial value for a range of the reported values for farinfrared and optical regimes^{68}. The absorption spectrum in our calculations was sampled with 2000 points in the energy range from 0 to 8 eV, which corresponds to the resolution of about 8 points per the Gaussian.
Fitting procedure
Using Quantum Espresso package, we calculated the DFT bandstructures for ZGNR\((6)\), \((9)\), \((12)\) and \((15)\). In each DFT bandstructure, only the \(\pi\)bands were selected for the fitting. The fitting was implemented on all valence \(\pi\)bands and several lowest conductions \(\pi\)bands: 6 valence and 2 conduction bands for ZGNR\((6)\), 9 valence and 3 conduction bands for ZGNR\((9)\), 12 valence and 4 conduction bands for ZGNR\((12)\) and 15 valence and 5 conduction bands for ZGNR\((15)\). The number of conduction bands was limited based on the pseudopotential vacuum level of about 4 eV; for fitting we chose only those conduction bands that lay below the vacuum level within the whole Brillouin zone. Each refined in this way DFT bandstructure was fitted with six parameters of TBM. In order to fit the six parameters \({\left\{{p}_{l}\right\}}_{l=1,\ldots ,6}=\{{t}_{1},{t}_{2},{t}_{3},{s}_{1},{s}_{2},{s}_{3}\}\), we minimized the following function:
where \({N}_{k}\) is the number of the Brillouin zone sampling points used in DFT calculations and \({N}_{{\rm{b}}}\) is the number of fitted bands. For the generalized eigenvalue problem \(H\Psi =ES\Psi\), the Hermiticity of \(H\) and \(S\) matrices is not a sufficient condition for having real eigenvalues. All real eigenvalues are guaranteed for \(H\Psi =ES\Psi\) problem only if \(S\) and \(H\) are not only Hermitian but also at least one of them is positive definite. This condition, however, is not fulfilled for many combinations of the hopping integrals varied between \(3\) and 3 eV and the overlapping integrals between \(1.5\) and 1.5. Therefore, to ensure realvaluedness of \(f(\left\{{p}_{l}\right\})\) and to exclude the sets of the tightbinding parameters resulting in complex eigenenegies, the sum of the squares of the deviations between the DFT and TBM energies in the first term of Eq. (3) is placed within a parabolic well described by the second term in Eq. (3). The mimimizations were performed in Mathematica 11.3.0 software based on its builtin NMinimize function designed to find the global minimum. Among the six methods given for this function, only the differential evolution method showed a steady convergence within \(< 200\) steps, i.e., for ZGNR(6) \(f{(\left\{{p}_{l}\right\})}_{\min }=1.6780\) eV\({}^{2}\) within 133 steps, for ZGNR(9) \(f{(\left\{{p}_{l}\right\})}_{\min }=2.7957\) eV\({}^{2}\) within 110 steps, for ZGNR(12) \(f{(\left\{{p}_{l}\right\})}_{\min }=3.5849\) eV\({}^{2}\) within 155 steps and for ZGNR(15) \(f{(\left\{{p}_{l}\right\})}_{\min }=4.4504\) eV\({}^{2}\) within 186 steps. The resulting parameters presented in Table 1 of the main text were then averaged over the four structures and were used in the TBM calculations for the ZGNRs. Before TBM optical absorption calculations, we checked that the found parameters provide a reasonable approximation to the DFT bandstructures (see Supplementary Figs. 1 and 2 in Supplementary Note 1).
Absorption resonance extraction
In each TBM absorption spectrum, the positions of the peaks were extracted using the algorithm (see Code Availability section) which identifies the positions of intensity maxima \({E}_{\max }\) for which the minimum intensity drop \(\Delta {I}_{\min }\) at the left or right boundary of the closed interval \(\left[{E}_{\max }dE,{E}_{\max }+dE\right]\) fulfills the following criterion:
where \(I(E)\) is the intensity of the interband absorption at a given energy and \(x\) is the threshold parameter measured in terms of percents.
In order to extract the significant peaks from the full and bulk ZGNR spectra in Patroens 2006 TBM, we used the following parameters in Eq. (4): \(x=8 \%\) and \(dE=0.07\) eV. To determine the peak positions for similar spectra calculated with ZGNR(av.) TBM presented in Table 1, we used \(x=4 \%\) and \(dE=0.1\) eV for both full and bulk absorption spectra. In the case of armchair SWCNTs, the optical absorption resonances were selected by the algorithm with \(x=19 \%\) and \(dE=0.1\) eV for Partoens 2006 and \(x=7\, \%\) and \(dE=0.05\) eV for Reich 2002 TBMs.
Linear correlation coefficient
The following modification of the standard formula [cf. Equation (7.18) in ref. ^{69}] for the linear correlation coefficient (LCC) calculation was used:
where \({N}_{x}\) and \({N}_{y}\) are the number of elements in datasets \(x\) and \(y\) representing the absorption resonances extracted from the spectra, while \(\bar{x}\) and \(\bar{y}\) are the mean values for the \(x\) and \(y\) datasets, respectively. In general, the numbers of resonances \({N}_{x}\) and \({N}_{y}\) in the absorption spectra of tubes and ribbons are different. Due to this reason, the summation in the numerator of Eq. (5) is defined for the less of \({N}_{x}\) and \({N}_{y}\). In this way, the LCC values were determined for all the combinations of tubes and ribbons of different transverse sizes and the LCC maps were generated.
Alignment coefficient or the likelihood function
The degree of alignment \({L}_{{\rm{c}}}\) between the two sets of resonances was described by the following alignment coefficient (AC) or the likelihood function, characterizing the average deviation of \({x}_{i}\) resonances from \({y}_{i}\) ones (cf. Equation (6.2) in ref. ^{69}):
where \(\beta =1\) eV\({}^{2}\) is a coefficient setting the energy units of \({x}_{i}\) and \({y}_{i}\) resonances and making the exponent dimensionless. Similar to the LCC, the AC defined by Eq. (6) truncates the dataset with a larger number of elements to the length of the smaller dataset, which allows one to generate the AC maps.
Data availability
The TBM and DFT calculations raw data that support the findings of this study are available in Zenodo with the identifier doi:10.5281/zenodo.3547546 or using link https://doi.org/10.5281/zenodo.3547546. This open access repository also contains Source Data files for Fig. 1 and Table 1. In addition, the repository contains scripts for performing the TBM calculations, TBM fitting and data analysis, including reproduction of Figs. 1–5 and Supplementary Figs. 1–8. These data and code can be alternatively obtained from the GitHub (see Code availability section). The data that support the findings of this study are also available from the corresponding author upon request.
Code availability
The code developed for this study is available under a GNU Lesser General Public License v3.0 from https://github.com/vasilsaroka/AnatlasofZGNRsbulkopticalresonances.
References
Areshkin, D. A. & White, C. T. Building blocks for integrated graphene circuits. Nano Lett. 7, 3253–3259 (2007).
Rao, R. et al. Carbon nanotubes and related nanomaterials: critical advances and challenges for synthesis toward mainstream commercial applications. ACS Nano 12, 11756–11784 (2018).
He, X. et al. Carbon nanotubes as emerging quantumlight sources. Nat. Mater. 17, 663–670 (2018).
Sun, Q., Zhang, R., Qiu, J., Liu, R. & Xu, W. Onsurface synthesis of carbon nanostructures. Adv. Mater. 30, 1705630 (2018).
Urgel, J. I. et al. Onsurface lightinduced generation of higher acenes and elucidation of their openshell character. Nat. Commun. 10, 861 (2019).
Janas, D. Towards monochiral carbon nanotubes: a review of progress in the sorting of singlewalled carbon nanotubes. Mater. Chem. Front. 2, 36–63 (2018).
Li, H., Gordeev, G., Garrity, O., Reich, S. & Flavel, B. S. Separation of smalldiameter singlewalled carbon nanotubes in one to three steps with aqueous twophase extraction. ACS Nano 13, 2567–2578 (2019).
Kataura, H. et al. Optical properties of singlewall carbon nanotubes. Synth. Met. 103, 2555–2558 (1999).
Weisman, R. B. & Bachilo, S. M. Dependence of optical transition energies on structure for singlewalled carbon nanotubes in aqueous suspension: an empirical Kataura plot. Nano Lett. 3, 1235–1238 (2003).
Araujo, P. T. et al. Third and fourth optical transitions in semiconducting carbon nanotubes. Phys. Rev. Lett. 98, 067401 (2007).
Liu, K. et al. An atlas of carbon nanotube optical transitions. Nat. Nanotechnol. 7, 325–329 (2012).
Wei, X. et al. Experimental determination of excitonic band structures of singlewalled carbon nanotubes using circular dichroism spectra. Nat. Commun. 7, 12899 (2016).
Yao, F. et al. Measurement of complex optical susceptibility for individual carbon nanotubes by elliptically polarized light excitation. Nat. Commun. 9, 3387 (2018).
Yanagi, K. et al. Intersubband plasmons in the quantum limit in gated and aligned carbon nanotubes. Nat. Commun. 9, 1121 (2018).
Gordeev, G., Flavel, B., Krupke, R., Kusch, P. & Reich, S. Asymmetry of resonance Raman profiles in semiconducting singlewalled carbon nanotubes at the first excitonic transition. Phys. Rev. B 99, 045404 (2019).
Satco, D. et al. Intersubband plasmon excitations in doped carbon nanotubes. Phys. Rev. B 99, 075403 (2019).
Michel, T. et al. E_{33} and E_{44} optical transitions in semiconducting singlewalled carbon nanotubes: electron diffraction and Raman experiment. Phys. Rev. B 75, 155432 (2007).
Popov, V. N. & Henrard, L. Comparative study of the optical properties of singlewalled carbon nanotubes within orthogonal and nonorthogonal tightbinding models. Phys. Rev. B 70, 115407 (2004).
Barone, V., Peralta, J. E., Wert, M., Heyd, J. & Scuseria, G. E. Density functional theory study of optical transitions in semiconducting singlewalled carbon nanotubes. Nano Lett. 5, 1621–1624 (2005).
Barone, V., Peralta, J. E. & Scuseria, G. E. Optical transitions in metallic singlewalled carbon nanotubes. Nano Lett. 5, 1830–1833 (2005).
Saroka, V. A., Batrakov, K. G., Demin, V. A. & Chernozatonskii, L. A. Band gaps in jagged and straight graphene nanoribbons tunable by an external electric field. J. Phys. Condens. Matter 27, 145305 (2015).
Beyer, D. et al. Graphene nanoribbons derived from zigzag edgeencased poly (para2,9dibenzo[bc,kl]coronenylene) polymer chains. J. Am. Chem. Soc. 141, 2843–2846 (2019).
Teeter, J. D. et al. Onsurface synthesis and spectroscopic characterization of laterally extended chevron graphene nanoribbons. Chem. Phys. Chem. 20, 2281–2285 (2019).
Sorokin, P. B. & Chernozatonskii, L. A. Graphenebased semiconductor nanostructures. PhysicsUspekhi 56, 105–122 (2013).
Palacio, I. et al. Atomic structure of epitaxial graphene sidewall nanoribbons: flat graphene, miniribbons, and the confinement gap. Nano Lett. 15, 182–189 (2015).
Baringhaus, J. et al. Growth and characterization of sidewall graphene nanoribbons. Appl. Phys. Lett. 106, 043109 (2015).
Lin, M.F. & Shyu, F.l Optical properties of nanographite ribbons. J. Phys. Soc. Japan 69, 3529–3532 (2000).
Chang, C. P. et al. Electronic and optical properties of a nanographite ribbon in an electric field. Carbon 44, 508–515 (2006).
Barone, V., Hod, O. & Scuseria, G. E. Electronic structure and stability of semiconducting graphene nanoribbons. Nano Lett. 6, 2748–2754 (2006).
Chung, H. C., Lee, M. H., Chang, C. P. & Lin, M. F. Exploration of edgedependent optical selection rules for graphene nanoribbons. Opt. Express 19, 23350–23363 (2011).
Sasaki, K.I., Kato, K., Tokura, Y., Oguri, K. & Sogawa, T. Theory of optical transitions in graphene nanoribbons. Phys. Rev. B 84, 085458 (2011).
Zhu, X. & Su, H. Scaling of excitons in graphene nanoribbons with armchair shaped edges. J. Phys. Chem. A 115, 11998–12003 (2011).
Jia, Y. L., Geng, X., Sun, H. & Luo, Y. Exciton effects in armchair graphene nanoribbons. Eur. Phys. J. B 83, 451–455 (2011).
Mohammadzadeh, L., Asgari, A., Shojaei, S. & Ahmadi, E. Theoretical calculation of excitonic binding energies and optical absorption spectra for armchair graphene nanoribbons. Eur. Phys. J. B 84, 249–253 (2011).
Lu, Y., Zhao, S., Lu, W., Liu, H. & Liang, W. Excitonic effects of E11, E22, and E33 in armchairedged graphene nanoribbons. J. Appl. Phys. 115, 103701 (2014).
Monozon, B. S. & Schmelcher, P. Exciton absorption spectra in narrow armchair graphene nanoribbons in an electric field. Phys. Rev. B 99, 165415 (2019).
Denk, R. et al. Excitondominated optical response of ultranarrow graphene nanoribbons. Nat. Commun. 5, 4253 (2014).
Borin Barin, G. et al. Surfacesynthesized graphene nanoribbons for room temperature switching devices: substrate transfer and ex situ characterization. ACS Appl. Nano Mater. 2, 2184–2192 (2019).
White, C. T., Li, J., Gunlycke, D. & Mintmire, J. W. Hidden oneelectron interactions in carbon nanotubes revealed in graphene nanostrips. Nano Lett. 7, 825–830 (2007).
Saroka, V. A., Pushkarchuk, A. L., Kuten, S. A. & Portnoi, M. E. Hidden correlation between absorption peaks in achiral carbon nanotubes and nanoribbons. J. Saudi Chem. Soc. 22, 985–992 (2018).
Portnoi, M. E., Saroka, V. A., Hartmann, R. R. & Kibis, O. V. in 2015 IEEE Comput. Soc. Annu. Symp. VLSI. pp. 456–459 (IEEE, Los Alamitos, CA, 2015).
Hartmann, R. R., Saroka, V. A. & Portnoi, M. E. Interband transitions in narrowgap carbon nanotubes and graphene nanoribbons. J. Appl. Phys. 125, 151607 (2019).
Shahnazaryan, V. A., Saroka, V. A., Shelykh, I. A., Barnes, W. L. & Portnoi, M. E. Strong lightmatter coupling in carbon nanotubes as a route to exciton brightening. ACS Photonics 6, 904–914 (2019).
Kivelson, S. & Chapman, O. L. Polyacene and a new class of quasionedimensional conductors. Phys. Rev. B 28, 7236–7243 (1983).
Tanaka, K., Yamashita, S., Yamabe, H. & Yamabe, T. Electronic properties of onedimensional graphite family. Synth. Met. 17, 143–148 (1987).
Fujita, M., Wakabayashi, K., Nakada, K. & Kusakabe, K. Peculiar localized state at zigzag graphite edge. J. Phys. Soc. Japan 65, 1920–1923 (1996).
Su, W. P., Schrieffer, J. R. & Heeger, A. J. Soliton excitations in polyacetylene. Phys. Rev. B 22, 2099–2111 (1980).
Tanikawa, Y., Suzuki, H. & Yomosa, S. Exact solutions of the secular equations in the HMO treatment for chain molecules of finite length. J. Phys. Soc. Japan 18, 1051–1056 (1963).
Jiang, J., Lu, W. & Bernholc, J. Edge states and optical transition energies in carbon nanoribbons. Phys. Rev. Lett. 101, 246803 (2008).
Yang, L., Cohen, M. L. & Louie, S. G. Magnetic edgestate excitons in zigzag graphene nanoribbons. Phys. Rev. Lett. 101, 186401 (2008).
Lu, Y., Lu, W., Liang, W. & Liu, H. Energy splitting and optical activation of triplet excitons in zigzagedged graphene nanoribbons. Phys. Rev. B 88, 165425 (2013).
Saroka, V. A., Shuba, M. V. & Portnoi, M. E. Optical selection rules of zigzag graphene nanoribbons. Phys. Rev. B 95, 155438 (2017).
Verzhbitskiy, I. A. et al. Raman fingerprints of atomically precise graphene nanoribbons. Nano Lett. 16, 3442–3447 (2016).
Hsu, H. & Reichl, L. E. Selection rule for the optical absorption of graphene nanoribbons. Phys. Rev. B 76, 045418 (2007).
Partoens, B. & Peeters, F. M. From graphene to graphite: electronic structure around the K point. Phys. Rev. B 74, 075404 (2006).
Lin, M. F. & Shung, K. W.K. Plasmons and optical properties of carbon nanotubes. Phys. Rev. B 50, 17744–17747 (1994).
Kravets, V. G. et al. Spectroscopic ellipsometry of graphene and an excitonshifted van Hove peak in absorption. Phys. Rev. B 81, 155413 (2010).
Mak, K. F., Shan, J. & Heinz, T. F. Seeing manybody effects in single and fewlayer graphene: observation of twodimensional saddlepoint excitons. Phys. Rev. Lett. 106, 046401 (2011).
Margaryan, N., Kokanyan, N. & Kokanyan, E. Lowtemperature synthesis and characteristics of fractal graphene layers. J. Saudi Chem. Soc. 23, 13–20 (2018).
Reich, S., Maultzsch, J., Thomsen, C. & Ordejón, P. Tightbinding description of graphene. Phys. Rev. B 66, 035412 (2002).
Saroka, V. Band structures in zigzag graphene nanoribbons and armchair carbon nanotubes; http://demonstrations.wolfram.com/BandStructuresInZigzagGrapheneNanoribbonsAndArmchairCarbonNa (2017).
Saroka, V. A. et al. Absorption in finitelength chevrontype graphene nanoribbons. Semiconductors 52, 1890–1893 (2018).
Talyzin, A. V. et al. Synthesis of graphene nanoribbons encapsulated in singlewalled carbon nanotubes. Nano Lett. 11, 4352–4356 (2011).
Chernov, A. I. et al. Optical properties of graphene nanoribbons encapsulated in singlewalled carbon nanotubes. ACS Nano 7, 6346–6353 (2013).
Chung, H.C., Chang, C.P., Lin, C.Y. & Lin, M.F. Electronic and optical properties of graphene nanoribbons in external fields. Phys. Chem. Chem. Phys. 18, 7573–7616 (2016).
Giannozzi, P. et al. Advanced capabilities for materials modelling with Quantum ESPRESSO. J. Phys. Condens. Matter 29, 465901 (2017).
Lew Yan Voon, L. C. & RamMohan, L. R. Tightbinding representation of the optical matrix elements: theory and applications. Phys. Rev. B 47, 15500–15508 (1993).
Shuba, M. V., Maksimenko, S. A. & Slepyan, G. Y. Absorption crosssection and nearfield enhancement in finitelength carbon nanotubes in the terahertztooptical range. J. Comput. Theor. Nanosci. 6, 2016–2023 (2009).
Bonamente, M. Statistics and analysis of scientific data p. 301 (Springer, New York, 2013).
Acknowledgements
The authors thank C.A. Downing, R.R. Hartmann, M.E. Portnoi, K.G. Batrakov, P.P. Kuzhir, A.L. Pushkarchuk, A.V. Kuhta, F. Yao and K. Liu for their very helpful discussions, J. Danon for providing computational facilities at NTNU and A.R. Villagracia for providing the computing workstation in STRC, De La Salle University. CPU time for the DFT calculations was granted by CINECA HPC center. This work was supported by EU H2020 RISE Project CoExAN (GA644076), and partly by the Research Council of Norway Center of Excellence funding scheme (project no. 262633, “QuSpin”). The authors also acknowledge the financial support from VCRI, De La Salle University.
Author information
Authors and Affiliations
Contributions
V.A.S. and D.I.L. conceived the idea. R.B.P. obtained the first DFT results. R.B.P., G.N.C.S., D.G. and O.P. performed DFT calculations on small and large structures and analysed the results. V.A.S. performed the fitting of TB models and TB calculations. D.I.L. and V.A.S. compared the results to the interpolation formulas for carbon nanotubes. V.A.S. and R.B.P. wrote the manuscript. All authors commented on the manuscript and assisted in revisions.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Peer review information Nature Communications thanks MingFa Lin and the other, anonymous, reviewer(s) for their contribution to the peer review of this work. Peer reviewer reports are available.
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Payod, R.B., Grassano, D., Santos, G.N.C. et al. 2N+4rule and an atlas of bulk optical resonances of zigzag graphene nanoribbons. Nat Commun 11, 82 (2020). https://doi.org/10.1038/s41467019137288
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41467019137288
This article is cited by

Terahertz radiation generation process in the medium based on the array of the elongated nanoparticles
Optical and Quantum Electronics (2022)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.